INFLUENCE KINDS OF MATERIALS ON THE POISSON S RATIO OF WOVEN FABRICS


 Marjory Cox
 1 years ago
 Views:
Transcription
1 ISSN (Print), ISSN (Online) ID: TG Original scientific paper INFLUENCE KINDS OF MATERIALS ON THE POISSON S RATIO OF WOVEN FABRICS Željko PENAVA, Diana ŠIMIĆ PENAVA, Željko KNEZIĆ Abstract: Poisson's ratio is one of the fundamental properties of any structural material including woven fabrics and textile materials. This coefficient determines important mechanical characteristics of fabrics in many applications, including a variety of composite systems containing textiles as a structural element. Due to the anisotropy of woven fabrics, Poisson's ratio changes over the fabric sample stretching. In this paper, the practical application of the uniaxial testing of woven fabrics for determining its breaking properties and Poisson's ratio is presented. Experimental testing was carried out on two different fabrics of a different raw material composition (, ) and of the same weave (plain weave). Samples were stretched with tensile force in the weft and warp direction, and based on the different measured values of the fabric stretching, warp and weft, Poisson's ratio is calculated. The influence of the raw material composition on the values of Poisson's ratio was examined. Keywords: anisotropy; elongation at break; Poisson s ratio; warp; weft; woven fabric 1 INTRODUCTION Nowadays, the use of textile materials in different industrial branches is on the rise. Anisotropy is a characteristic of most materials, especially woven fabrics. The impact of the direction of action of the external load (tensile force) on the properties of the fabric is enormous, and is frequently examined [1]. The mechanical properties of fabrics under the influence of the tensile load began to be studied in 1937 [2]. Kilby defined the Poisson's ratio and measured the tensile properties of fabrics in an arbitrary direction of the tensile force. He noted that there is a connection between the Poisson's ratio, shear modulus and modulus of the elasticity of the fabric [3]. The Poisson's ratio affects certain mechanical properties of the fabric such as the draping and shear. The researchers determined Poisson's ratio in the warp and weft based on the geometric model of fabric and without the impact of the Poisson's ratio of the yarn. The Poisson's ratio in fabrics comes out of the interaction between the warp and weft, and can be expressed in terms of structural and mechanical system parameters [4]. Due to the woven fabric anisotropy, the analysis of the impact of the physical parameters of fabric on the value of the Poisson's ratio is useful and provides a better explanation for certain woven fabric behavior. Because of the inherent nature of textile, an accurate and reliable measurement of the Poisson's ratio is a difficult task. This engineering property is studied by many scientists. Bao and colleagues [5] were examining why in the measurements of the Poisson's ratio, when uniaxial tensile load is put on the fabric, errors occur. The previously measured experimental values were compared with the theoretical results. He also studied the influence of the yarn and fabric structural parameters of the Poisson's ratio. An accurate measurement of the Poisson's ratio of woven fabric is quite difficult to obtain due to the lack of reliable experimental techniques [6]. Uniaxial testing is most commonly performed in woven fabrics by using either the commercial or custom designed instruments [7] and analyzing the physical and mechanical properties of textile products [8]. The Poisson's ratio of textile materials used in the nonwoven geotextile was analyzed by Giroud [9]. He set the theoretical equation to calculate the Poisson coefficient, as a function of strain. Experiments on the extension of the woven fabric sample under the static load will are discussed in this paper. The influence of the raw material composition on the values of the Poisson's ratio has been researched, too. 2 THEORETICAL OVERVIEW The Poisson's ratio, which expresses the change in the volume of a solid undergoing deformation, is an important characteristic, along with the initial modulus of elasticity and shear, of the behavior of a material under a tension load; and can be used in the calculations of the true stresses (from the actual crosssectional area) coming into being in the textile fibers and yarns subjected to the extension, and can serve, moreover, as an indirect characteristic of the structure of the material and of the mechanism of its deformation. It is well known that when a solid having the shape of a rectangular parallelepiped, Fig. 1a, is subjected to tension forces in the direction of its axes x, y and z, the change in its volume equals: dv y z d x x z d y x y d V x y z d d x y d z x y z x y z where ε x, ε y and ε z are the relative tensile deformations in the direction of the x, y and z axes of the parallelepiped. z (1) TEHNIČKI GLASNIK 11, 3(217),
2 dx L z dy s y (1+ y )dy L d x x T (1+ y )d y s x s x d y T y s y (1+ x )dx (1+ x )d x a) b) c) Figure 1 Schematic presentation of: a) solid volume element, b) Poisson s ratio ν xy, c) Poisson s ratio ν yx In the tensile deformation in the direction of the x axis, the solid will be subjected to compression in the direction of the y and z axes (i.e, laterally to the x axis): dv V x 2 x 1 2 x 1 2 x where ε is the relative compressive deformation and ν is the Poisson s ratio. It is obvious that for ν =.5 the volume of a material subjected to tensile forces will not change (dv = ), for ν <.5 the volume will increase (dv > ), while for ν >.5 it will decrease (dv < ). When a fabric is stretched in one direction, it tends to contract in the direction perpendicular to the direction of the stretch, Fig. 1b, 1c. The yarns in the direction of the tensile force are flattened out (extended), and in the orthogonal or nonloading direction, the yarns have a longer geometrical path to 'curve around'. Because there is no limiting force, the waviness (amplitude) of the yarn in the vertical direction of the force increases. The consequence to this is the dimension reduction of the fabric width. This phenomenon is called the Poisson effect. The Poisson s ratio, a measure of the Poisson effect, is the ratio of the relative contraction strain s to the related extension strain ε in the direction of the applied load. To determine the Poisson's ratio of fabrics, devices for measuring the tensile strength are used, and the coefficient is determined in the linear part of the diagram of the Hooke's law [1]. During the testing of the fabric to stretch, the initial length of the tested sample l is increased for Δl, and a final sample length of fabric is l. The initial width of the fabric sample b is decreased for Δb and the final sample width is b. The physical meaning of the Poisson's ratio ν is shown by the Eq. (3). The Relative contraction and extension strains have an opposite sign. (2) s l b b, b l l s. (3) The relative longitudinal strain (relative extension strain) ε and transverse strain (relative contraction strain) s is defined in the Eq. (4). l l 1% 1 1% l l. (4) b b s 1% 11% b b Due to the anisotropy of the fabric, the Poisson s ratio is being changed in the process of the extension of the fabric sample. 3 EXPERIMENTAL TESTING The experimental study was carried out by measuring the extension of woven fabrics samples under the action of the tensile force till rupture [11]. The tensile force acts on the samples that are cut at warp and weft direction. The values of the tensile force in relation to the relative extension were measured. For the extensions and tensile forces which act in the warp and weft direction, the corresponding contraction strains of woven fabrics were scanned. The Poisson's ratio of woven fabrics was calculated by using the testing results. Two different fabrics of a different raw material composition (, ) and of the same weave (plain weave) were available. The raw material and the structural properties of the tested fabrics are shown in Tab. 1. Table 1 Structural characteristics of the tested samples Warp direction Weft direction Fabric structure Fiber Yarn count Linera density Fiber Linera density Mass per unit Thickness, t composition (tex) (cm 1 Yarn count (tex) ) composition (cm 1 ) area (g/m 2 ) (mm) Plain Cotton Cotton Plain Wool Wool TECHNICAL JOURNAL 11, 3(217), 1116
3 The yarn count was determined by the gravimetric method according to the standard ISO 26:1994. The number of threads per unit length was tested according to the standard ISO :1984. The standard ISO 584:1996 describes a method for the determination of the thickness of the fabric. Before testing all samples were conditioned under the conditions of the standard atmosphere (relative air humidity 65 ± 2 %, at a temperature of 2 ± 2 C). Standard samples with the dimensions of 3 5 mm were cut and clamped in clamps of the tensile tester at a distance of l =2 mm and subjected to a uniaxial tensile load till rupture. The pulling speed of clamps is 1 mm/min. The samples were cut in the weft direction (φ = ) and warp direction (φ = 9 ). Three tests were done on the tensile tester for each mentioned cutting direction of the sample. The tensile properties of all samples were tested in accordance with the standard ISO ISO :28 by using the strip method for measuring the fabric strength on the tensile strength tester Textechno Statimat M. This tensile tester is an automatic, microprocessorcontrolled instrument operating on the principle of constant deformation speed, Fig. 2. Textechno sample sync on/off Figure 2 Schematic view of the experiment CAMERA SOFTWARE STATIMAT M SOFTWARE For an accurate recording and measurement of the spatial deformation of fabric, a 1x1 grid pattern was mounted on the tensile tester immediately behind the test specimen; the whole process of drawing the specimen till rupture was recorded by the Panasonic NVGS5 Digital Video Camera placed on a tripod in front of the device. The digital video camera had the resolution of pixels, and a recording speed of N sl=25 frames/s, and was connected to the computer via an IEEE 1394 (FireWire) interface. The horizontal distance between the camera and the sample was such that 1 mm on the grid amounted to 1 pixels on the picture. Two sources of white light which mutually closed the angle of 9 were used for measuring. The number of images N at a certain extension is: l 6 N Nsl. (5) 1 v The tensile tester and the camera were connected to a special assembly with a simultaneous on/off which fully ensured the exactness of the video recording of the entire process of stretching the fabric to rupture. The width of each sample was measured in three spots (1/4, 2/4 and 3/4 of the length and width of the sample). The transverse strain was obtained after all samples were recorded by camera, and the mentioned grid pattern enabled a fast and accurate editing of the footage processed by the software package Adobe Premiere created for this purpose which specified the spatial deformation of samples on the basis of shifting in the direction of the x and yaxis. 3.1 Overview of testing results The diagrams (Fε) of mean values of the test results of the action of the tensile force F and the corresponding longitudinal strain (extension) ε for the samples that are cut in the weft and warp direction are shown in Fig F (N) 3 F (N) a) b) Figure 3 Tensile forceelongation diagram (Fε) till rupture: a) when the force acts in the weft direction, b) when the force acts in the warp direction TEHNIČKI GLASNIK 11, 3(217),
4 3.2 Determination of Poisson's ratio The fabric sample width is b = 5 pixels, which is equivalent to b = 5 mm. When reading the value of the fabric width, after the effect of the force, the relative transverse strain is calculated by using the Eq. (4). The contraction of fabric occurs in the transverse direction, i.e. in the direction which is perpendicular to the direction of stretching. Due to this phenomenon, there is a loss of the rectangular shape of the sample, i.e. there is a contraction of the fabric sample. The relation between the continuous change of the relative contraction s (%) of the sample and its relative extension when a force acts on the samples that are cut in the weft direction is shown in Fig. 4a by a characteristic curve. Fig. 4b shows a characteristic curve of the relative contraction of the sample in relation to its relative extension when the force acts on samples that are cut in the warp direction. When a force acts on samples that are cut in the weft and warp direction, at the same relative extension ε, fabric has a higher relative contraction s than fabric, Fig. 4. When the force acts in the weft direction, at a relative extension ε = 1%, the lateral contraction for the fabric is s = 12.56% and for fabric s = 7.57 %. The lateral contraction of fabric is 66% higher than the contraction of fabrics for ε = 1%. When force acts in the warp direction, at a relative extension ε = 15.5%, the lateral contraction for fabric is s = 17.47% and for fabric s = 9.12%. The lateral contraction of fabric is 92% higher than the contraction of fabric for ε = 15.5%. Both fabrics have a bigger extension and contraction when the force acts in the warp direction s (%) 68 s (%) a) b) Figure 4 Diagram of the relative contraction of the fabric s (%): a) when the force acts in the weft direction, b) when the force acts in the warp direction 2 From the diagrams in Fig. 4 it is evident that fabric contractions are small at the beginning of stretching. After that, with the increase of stretching, the values of fabric contractions also increase. According to the Eq. (3) and based on the experimental values of the relative contraction s and relative extension ε from Fig. 4, the values of the Poisson s ratio v are calculated when the force acts on the samples that are cut in the weft and warp direction. Fig. 5a shows a curve of the values of the Poisson s ratio v in relation to its relative extension when the force acts on the samples that are cut in the weft direction and Fig. 5b shows the values in the warp direction a) b) Figure 5 Poisson s ratio v of the fabric: a) when the force acts in the weft direction, b) when the force acts in the warp direction 14 TECHNICAL JOURNAL 11, 3(217), 1116
5 The shape of the Poisson s ratio curve of the woven fabric is the result of the internal interactions in the fabric. The shape of the Poisson s ratio (Fig. 5) affected by the changes in the value of the relative contraction of the fabric are shown in Fig. 4. The Poisson s ratio curve consists of two zones. The first zone includes the area from the beginning to the highest peak of the curve. When a force acts in the weft direction, the highest value of the Poisson s ratio for the fabric ν = 1.39 is where the relative extension ε is between 6 and 6.5%, and for fabric ν =.88 is where ε is between 5.5 and 6%, Fig. 5a. When a force acts in the warp direction, the highest value of the Poisson s ratio for the fabric ν = 1.18 is where the relative extension ε is between 14 and 14.5%, and for fabric ν =.68 is where ε is between 9.5 and 1%, Fig. 5b. Both fabrics have a higher value of the Poisson s ratio when the force acts in the weft direction. Cotton fabric has a higher value of the Poisson s ratio than fabric for each value of the extension. When the force acts in the weft direction, at a relative extension ε = 6 %, the value of the Poisson s ratio for fabric is 62% higher than the Poisson s ratio for fabrics. When the force acts in the warp direction, at a relative extension ε = 6 %, the value of Poisson s ratio for fabric is 52% higher than the Poisson s ratio for fabrics. The second zone is from the highest peak of the curve to the end of stretching, i.e. it is interrupted. In this zone, the curve of the Poisson s ratio decreases and it represents the end of the lateral contraction despite the stretching of the fabric sample. After considering the equation of the Poisson s ratio, the relative contraction becomes a constant when the lateral contraction of the woven fabric is completed. Furthermore, the sample is still stretching for the value ε. Therefore, the equation of the Poisson s ratio takes on a new form, which is the general form of the reciprocal function. Mathematically, the limit of this equation is zero. In practice, due to the break of the sample, this condition never occurs. However, taking into account the significance of the Poisson s ratio that represents the ratio between the transverse and longitudinal deformation of the material, if the transverse deformation does not take place in this ratio, the Poisson s ratio has no practical significance. The ending of the lateral contraction of a woven fabric can occur for two reasons. Firstly, due to the termination of the flattening crimp of yarn in the direction of the stretching fabric and secondly, because of the structure of the fabric. If there is a possibility of a further contraction of fabric, it can not continue taking place because there is no continued existence of space between the neighboring threads in the fabric, so there can be no contraction of the fabric. Note: This research was presented at the International Conference MATRIB 217 (29 June  2 July 217, Vela Luka, Croatia). 4 CONCLUSION Due to the anisotropy of woven fabrics, the Poisson's ratio is not constant, but varies with each fabric extension. The behavior and shape of the Poisson s ratio curve of the coated fabric that is subjected to the tensile force mostly depends on its behavior in a direction perpendicular to the extension. The Poisson s ratio values depend on the number of coatings applied to the raw fabric. The shape of the Poisson s ratio curve for woven fabrics is a result of the internal interactions in the coated and raw fabrics. A change in the values of the relative contraction of coated fabrics affects the shape of the Poisson s ratio curve. When the force acts on samples that are cut in the weft direction, the Poisson's ratio assumes the maximum value at a relative extension of fabrics between 6 and 6.5%, and for fabrics between 5 and 5.5%. When the force acts on the samples that are cut in the warp direction, the Poisson s ratio assumes the maximum value at a relative extension of fabrics between 14 and 14.5%, and between 9.5 and 1% for fabrics. In the weft and warp direction, the values of the Poisson s ratio of fabrics are higher than the Poisson s ratio of fabrics at the same relative extension. Because of the anisotropy of fabrics, the Poisson s ratio is not constant. It is changing with each elongation of the woven fabric. The behavior and form of the curve of the Poisson s ratio of the woven fabric which is exposed to tensile force, i.e. elongation, mainly depends on the behavior of the fabric in a direction perpendicular to the elongation. First, the Poisson s ratio increases nonlinearly and after having reached the peak value, it decreases. These two zones represent two different processes in the deformation of the fabric. The first zone represents the way of the lateral contraction because of the longitudinal stretching. The second zone shows the termination of the lateral contraction of the woven fabric and the fabric is stretching without any further contractions. 5 REFERENCES [1] Kovar, R.; Gupta, B. S. Study of the Anisotropic Nature of the Rupture Properties of a Plain Woven Fabric. // Textile Research Journal, 79, 6(29), pp [2] Peirce, F. T. The geometry of cloth structure. // Journal of the Textile Institute, 28, (1937), T45T96. [3] Kilby, W. F. Planar Stressstrain Relationship in Woven Fabrics. // Journal of the Textile Institute, 54, (1963), pp [4] Lloyd, D. W. et al. An Examination of a "Wide jaw" Test for the Determination of Fabric Poisson Ratio. // Journal of the Textile Institute, 68, 9(1977), pp [5] Bao, L. et al. Error Evaluation in Measuring the Apparent Possion s Ratios of Textile Fabrics by Uniaxial Tensile Test. // Sen i Gakkaishi, 53, 1(1997), pp TEHNIČKI GLASNIK 11, 3(217),
6 [6] Basset, R. J. et al. Experiment Methods for Measuring Fabric Mechanical Properties: a Review and Analysis. // Textile Research Journal, 69, 11(1999), pp [7] Sun, H. On the Poisson's ratios of a woven fabric. // Composite Structures, 68, 4(25), pp [8] Zheng, J. Measuring Technology of the Anisotropic Tensile Properties of Woven Fabrics. // Textile Research Journal, 78, 12(28), pp [9] Giroud, J. P. Poisson's Ratio of Unreinforced Geomembranes and Nonwoven Geotextiles Subjected to Large Strains. // Geotextiles and Membrane, 22, (24), pp [1] Nazanin, E. S. et al. Effect of Fabric Structure and Weft Density on the Poisson s Ratio of Worsted Fabric. // Journal of Engineered Fibers and Fabrics, 8, 2(213), pp [11] Penava, Ž. et al. Investigation of warp and weft takeup influence on Poisson's ratio of woven fabric. // Tekstil, 63, 78(214), pp Authors contacts: Željko PENAVA University of Zagreb, Faculty of Textile Technology, Prilaz B. Filipovića 28a, 1 Zagreb, Croatia Diana ŠIMIĆ PENAVA University of Zagreb, Faculty of Civil Engineering, Kačićeva 26, 1 Zagreb, Croatia Željko KNEZIĆ University of Zagreb, Faculty of Textile Technology, Prilaz B. Filipovića 28a, 1 Zagreb, Croatia 16 TECHNICAL JOURNAL 11, 3(217), 1116
EXPERIMENTAL ANALYSIS OF THE TENSILE PROPERTIES OF PAINTING CANVAS
AUTEX Research Journal, DOI: 1.1515/aut21523 AUTEX EXPERIMENTAL ANALYSIS OF THE TENSILE PROPERTIES OF PAINTING CANVAS Željko Penava 1 *, Diana Šimić Penava 2, Marijana Tkalec 1 1 University of Zagreb,
More informationThe influence of fiber undulation on the mechanical properties of FRPlaminates. Christian Fiebig, Michael Koch
URN (Paper): urn:nbn:de:gbv:ilm12014iwk099:3 58 th ILMENAU SCIENTIFIC COLLOQUIUM Technische Universität Ilmenau, 08 12 September 2014 URN: urn:nbn:de:gbv:ilm12014iwk:3 The influence of fiber undulation
More informationINTRODUCTION TO STRAIN
SIMPLE STRAIN INTRODUCTION TO STRAIN In general terms, Strain is a geometric quantity that measures the deformation of a body. There are two types of strain: normal strain: characterizes dimensional changes,
More informationModule III  Macromechanics of Lamina. Lecture 23. MacroMechanics of Lamina
Module III  Macromechanics of Lamina Lecture 23 MacroMechanics of Lamina For better understanding of the macromechanics of lamina, the knowledge of the material properties in essential. Therefore, the
More informationLab Exercise #5: Tension and Bending with Strain Gages
Lab Exercise #5: Tension and Bending with Strain Gages Prelab assignment: Yes No Goals: 1. To evaluate tension and bending stress models and Hooke s Law. a. σ = Mc/I and σ = P/A 2. To determine material
More information6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa ( psi) and
6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa (15.5 10 6 psi) and an original diameter of 3.8 mm (0.15 in.) will experience only elastic deformation when a tensile
More informationME 243. Mechanics of Solids
ME 243 Mechanics of Solids Lecture 2: Stress and Strain Ahmad Shahedi Shakil Lecturer, Dept. of Mechanical Engg, BUET Email: sshakil@me.buet.ac.bd, shakil6791@gmail.com Website: teacher.buet.ac.bd/sshakil
More informationBIAS EXTENSION TEST STANDARD
BIAS EXTENSION TEST STANDARD Xiongqi Peng and Jian Cao Advanced Materials Processing Laboratory Department of Mechanical Engineering Northwestern University Evanston, IL August 2003 For Internal Use 1.
More informationMeasurement of mesoscale deformations for modelling textile composites
CompTest 2004 Measurement of mesoscale deformations for modelling textile composites P Potluri, D A Perez Ciurezu, R Ramgulam Textile Composites Group University of Manchester Institute of Science & Technology
More information**********************************************************************
Department of Civil and Environmental Engineering School of Mining and Petroleum Engineering 333 Markin/CNRL Natural Resources Engineering Facility www.engineering.ualberta.ca/civil Tel: 780.492.4235
More informationStressStrain Behavior
StressStrain Behavior 6.3 A specimen of aluminum having a rectangular cross section 10 mm 1.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.
More information3. BEAMS: STRAIN, STRESS, DEFLECTIONS
3. BEAMS: STRAIN, STRESS, DEFLECTIONS The beam, or flexural member, is frequently encountered in structures and machines, and its elementary stress analysis constitutes one of the more interesting facets
More information4.MECHANICAL PROPERTIES OF MATERIALS
4.MECHANICAL PROPERTIES OF MATERIALS The diagram representing the relation between stress and strain in a given material is an important characteristic of the material. To obtain the stressstrain diagram
More informationSHEAR TENSION COUPLING IN BIAXIAL BIAS EXTENSION TESTS
SHER TENSION COUPLING IN IXIL IS EXTENSION TESTS P. Harrison *, P. Potluri Department of Mechanical Engineering, James Watt uilding (South), University of Glasgow, Glasgow G 8QQ, U.K. p.harrison@mech.gla.ac.uk
More informationNORMAL STRESS. The simplest form of stress is normal stress/direct stress, which is the stress perpendicular to the surface on which it acts.
NORMAL STRESS The simplest form of stress is normal stress/direct stress, which is the stress perpendicular to the surface on which it acts. σ = force/area = P/A where σ = the normal stress P = the centric
More informationCHAPTER 6 BENDING Part 1
Ishik University / Sulaimani Civil Engineering Department Mechanics of Materials CE 211 CHAPTER 6 BENDING Part 11 CHAPTER 6 Bending Outlines of this chapter: 6.1. Chapter Objectives 6.2. Shear and
More informationEvaluation of inplane orthotropic elastic constants of paper and paperboard
Evaluation of inplane orthotropic elastic constants of paper and paperboard T. Yokoyama and K. Nakai Department of Mechanical Engineering, Okayama University of Science  Ridaicho, Okayama 75, Japan
More information[8] Bending and Shear Loading of Beams
[8] Bending and Shear Loading of Beams Page 1 of 28 [8] Bending and Shear Loading of Beams [8.1] Bending of Beams (will not be covered in class) [8.2] Bending Strain and Stress [8.3] Shear in Straight
More informationEMA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading
MA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading MA 3702 Mechanics & Materials Science Zhe Cheng (2018) 2 Stress & Strain  Axial Loading Statics
More informationSTRAIN. Normal Strain: The elongation or contractions of a line segment per unit length is referred to as normal strain denoted by Greek symbol.
STRAIN In engineering the deformation of a body is specified using the concept of normal strain and shear strain whenever a force is applied to a body, it will tend to change the body s shape and size.
More informationSupplementary Information. Multifunctional graphene woven fabrics
Supplementary Information Multifunctional graphene woven fabrics Xiao Li 1, Pengzhan Sun 1, Lili Fan 1, Miao Zhu 1,2, Kunlin Wang 1, Dehai Wu 1, Yao Cheng 2,3 and Hongwei Zhu 1,2* 1 Department of Mechanical
More informationELASTICITY (MDM 10203)
ELASTICITY () Lecture Module 3: Fundamental Stress and Strain University Tun Hussein Onn Malaysia Normal Stress inconstant stress distribution σ= dp da P = da A dimensional Area of σ and A σ A 3 dimensional
More informationPrediction of Elastic Constants on 3D Fourdirectional Braided
Prediction of Elastic Constants on 3D Fourdirectional Braided Composites Prediction of Elastic Constants on 3D Fourdirectional Braided Composites Liang Dao Zhou 1,2,* and Zhuo Zhuang 1 1 School of Aerospace,
More informationDEVELOPMENT OF THE MEASURING SYSTEM FOR ANALYSING THE THERMAL PROPERTIES OF CLOTHING
DEVELOPMENT OF THE MEASURING SYSTEM FOR ANALYSING THE THERMAL PROPERTIES OF CLOTHING Dubravko ROGALE; Snježana FIRŠT ROGALE & Ivana ŠPELIĆ Abstract:The measuring system for assessing static and dynamic
More informationDRAPING SIMULATION. Recent achievements and future trends. Dr. Sylvain Bel LGCIE University Lyon 1
DRAPING SIMULATION Recent achievements and future trends 1 Dr. Sylvain Bel LGCIE University Lyon 1 2 DRAPING SIMULATION Why? How? What? DRAPING SIMULATION WHY? Clamps Punch Fabric Die 1 2 Resin 3 4 Fig.
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationNonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. F Talence, France Le Cheylard, France
20 th International Conference on Composite Materials Copenhagen, 1924th July 2015 Nonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. Thierry Lorriot 1, Jalal El Yagoubi
More informationFailure analysis of serial pinned joints in composite materials
Indian Journal of Engineering & Materials Sciences Vol. 18, April 2011, pp. 102110 Failure analysis of serial pinned joints in composite materials Alaattin Aktaş* Department of Mechanical Engineering,
More informationFAVIMAT (AI)ROBOT2 FAVIGRAPH. Automatic SingleFibre Testers
FAVIMAT (AI)ROBOT2 FAVIGRAPH Automatic SingleFibre Testers SingleFibre Testers FAVIMAT and FAVIGRAPH The FAVIMAT testing methods Testing and evaluation of a wide range of fibre properties are essential
More information[5] Stress and Strain
[5] Stress and Strain Page 1 of 34 [5] Stress and Strain [5.1] Internal Stress of Solids [5.2] Design of Simple Connections (will not be covered in class) [5.3] Deformation and Strain [5.4] Hooke s Law
More informationMECE 3321 MECHANICS OF SOLIDS CHAPTER 3
MECE 3321 MECHANICS OF SOLIDS CHAPTER 3 Samantha Ramirez TENSION AND COMPRESSION TESTS Tension and compression tests are used primarily to determine the relationship between σ avg and ε avg in any material.
More informationPRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses
OPTIMAT BLADES Page 1 of 24 PRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses first issue Peter Joosse CHANGE RECORD Issue/revision date pages Summary of changes draft 241002
More informationStudy on the Bursting Strength of Jute Fabric Asis Mukhopadhyay 1, Biwapati Chatterjee 2, Prabal Kumar Majumdar 3 1 Associate Professor,
American International Journal of Research in Science, Technology, Engineering & Mathematics Availale online at http://www.iasir.net ISSN (Print): 383491, ISSN (Online): 383580, ISSN (CDROM): 38369
More informationEXPERIMENTAL EVALUATION OF SHEAR STRENGTH OF WOVEN WEBBINGS
EXPERIMENTAL EVALUATION OF SHEAR STRENGTH OF WOVEN WEBBINGS Kevin L. Peil +, Ever J. Barbero +, Eduardo M. Sosa* + Department of Mechanical and Aerospace Engineering, West Virginia University (WVU), Morgantown,
More informationMechanical Behavior of Composite Tapered Lamina
International Journal of Engineering Research and Development eissn: 2278067X, pissn: 2278800X, www.ijerd.com Volume 10, Issue 8 (August 2014), PP.1927 Mechanical Behavior of Composite Tapered Lamina
More informationMaterial testing method for understanding rubber s mechanical characteristics QuasiStatic Tension Test
Material testing method for understanding rubber s mechanical characteristics QuasiStatic ension est 1 Introduction In this working group, we conduct tension tests of rubber materials to characterize
More informationPURE BENDING. If a simply supported beam carries two point loads of 10 kn as shown in the following figure, pure bending occurs at segment BC.
BENDING STRESS The effect of a bending moment applied to a crosssection of a beam is to induce a state of stress across that section. These stresses are known as bending stresses and they act normally
More informationMULTISCALE MODELLING OF FIBRE BUNDLES
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MULTISCALE MODELLING OF FIBRE BUNDLES N. D. Chakladar 1, P. Mandal 1 *, P. Potluri 2 1 School of Mechanical, Aerospace and Civil Engineering,
More informationFlexural properties of polymers
A2 _EN BUDAPEST UNIVERSITY OF TECHNOLOGY AND ECONOMICS FACULTY OF MECHANICAL ENGINEERING DEPARTMENT OF POLYMER ENGINEERING Flexural properties of polymers BENDING TEST OF CHECK THE VALIDITY OF NOTE ON
More informationINVESTIGATION OF THE PROCESSING PARAMETERS OF A 3D WOVEN REINFORCEMENT
INVESTIGATION OF THE PROCESSING PARAMETERS OF A 3D WOVEN REINFORCEMENT Andreas Endruweit, Dhiren K. Modi and Andrew C. Long School of Mechanical, Materials and Manufacturing Engineering, University of
More informationBioMechanics and BioMaterials Lab (BME 541) Experiment #5 Mechanical Prosperities of Biomaterials Tensile Test
BioMechanics and BioMaterials Lab (BME 541) Experiment #5 Mechanical Prosperities of Biomaterials Tensile Test Objectives 1. To be familiar with the material testing machine(810le4) and provide a practical
More informationMECHANICS OF MATERIALS
Third E CHAPTER 2 Stress MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Texas Tech University and Strain Axial Loading Contents Stress & Strain:
More informationME 2570 MECHANICS OF MATERIALS
ME 2570 MECHANICS OF MATERIALS Chapter III. Mechanical Properties of Materials 1 Tension and Compression Test The strength of a material depends on its ability to sustain a load without undue deformation
More informationActa Materiae Compositae Sinica Vol123 No12 April 2006
Acta Materiae Compositae Sinica Vol123 No12 April 2006 : 1000 3851 (2006) 02 0059 06 23 2 4 2006 3, (, 300160) :, 4 / 3D 2 0 30 45 60 90 :,, ; 4,, ;,, : ; ; : TB332 ; V258. 3 : A Mechanical anisotropy
More informationENGN 2340 Final Project Report. Optimization of Mechanical Isotropy of Soft Network Material
ENGN 2340 Final Project Report Optimization of Mechanical Isotropy of Soft Network Material Enrui Zhang 12/15/2017 1. Introduction of the Problem This project deals with the stressstrain response of a
More informationSamantha Ramirez, MSE. Stress. The intensity of the internal force acting on a specific plane (area) passing through a point. F 2
Samantha Ramirez, MSE Stress The intensity of the internal force acting on a specific plane (area) passing through a point. Δ ΔA Δ z Δ 1 2 ΔA Δ x Δ y ΔA is an infinitesimal size area with a uniform force
More informationAN LSDYNA USER DEFINED MATERIAL MODEL FOR LOOSELY WOVEN FABRIC WITH NONORTHOGONAL VARYING WEFT AND WARP ANGLE
7 th International LSDYNA Users Conference Material Technology (1) AN LSDYNA USER DEFINED MATERIAL MODEL FOR LOOSELY WOVEN FABRIC WITH NONORTHOGONAL VARYING WEFT AND WARP ANGLE Marlin Brueggert Romil
More informationAnalytical Modeling of the StressStrain Distribution in a Multilayer Structure with Applied Bending
Analytical Modeling of the StressStrain Distribution in a Multilayer Structure with Applied Bending Ana Neves Vieira da Silva Prof. Doutora Susana Isabel Pinheiro Cardoso de Freitas Dep. Physics, IST,
More informationMESOSCALE MODELLING IN THERMOPLASTIC 5HARNESS SATIN WEAVE COMPOSITE
MESOSCALE MODELLING IN THERMOPLASTIC 5HARNESS SATIN WEAVE COMPOSITE S. Daggumati a*,i. De Baere a, W. Van Paepegem a, J. Degrieck a, J. Xu b, S.V. Lomov b, I. Verpoest b a Ghent University, Dept. of
More informationStandard Test Method for Tensile Properties of Geotextiles by the WideWidth Strip Method 1
Designation: D 4595 09 Standard Test Method for Tensile Properties of Geotextiles by the WideWidth Strip Method 1 This standard is issued under the fixed designation D 4595; the number immediately following
More informationMicromeso draping modelling of noncrimp fabrics
Micromeso draping modelling of noncrimp fabrics Oleksandr Vorobiov 1, Dr. Th. Bischoff 1, Dr. A. Tulke 1 1 FTA Forschungsgesellschaft für Textiltechnik mbh 1 Introduction Noncrimp fabrics (NCFs) are
More informationInternational Journal of Scientific & Engineering Research, Volume 5, Issue 1, January ISSN
International Journal of Scientific & Engineering Research, Volume 5, Issue 1, January214 29 An Experimental Analysis of Stress Relaxation in Nonwoven Fabrics Sajid Ahmed Qureshi ABSTRACT  The current
More informationMECHANICS OF MATERIALS. Analysis of Beams for Bending
MECHANICS OF MATERIALS Analysis of Beams for Bending By NUR FARHAYU ARIFFIN Faculty of Civil Engineering & Earth Resources Chapter Description Expected Outcomes Define the elastic deformation of an axially
More information3.032 Problem Set 2 Solutions Fall 2007 Due: Start of Lecture,
3.032 Problem Set 2 Solutions Fall 2007 Due: Start of Lecture, 09.21.07 1. In the beam considered in PS1, steel beams carried the distributed weight of the rooms above. To reduce stress on the beam, it
More informationChapter 6: Mechanical Properties of Metals. Dr. Feras Fraige
Chapter 6: Mechanical Properties of Metals Dr. Feras Fraige Stress and Strain Tension Compression Shear Torsion Elastic deformation Plastic Deformation Yield Strength Tensile Strength Ductility Toughness
More informationSTANDARD SAMPLE. Reduced section " Diameter. Diameter. 2" Gauge length. Radius
MATERIAL PROPERTIES TENSILE MEASUREMENT F l l 0 A 0 F STANDARD SAMPLE Reduced section 2 " 1 4 0.505" Diameter 3 4 " Diameter 2" Gauge length 3 8 " Radius TYPICAL APPARATUS Load cell Extensometer Specimen
More informationRELATIONSHIP BETWEEN RADIAL COMPRESSIVE MODULUS OF ELASTICITY AND SHEAR MODULUS OF WOOD Jen Y. Liu Research Engineer
RELATIONSHIP BETWEEN RADIAL COMPRESSIVE MODULUS OF ELASTICITY AND SHEAR MODULUS OF WOOD Jen Y. Liu Research Engineer and Robert J. Ross Supervisory Research Engineer USDA Forest Service Forest Products
More informationElastic Properties of Solids (One or two weights)
Elastic properties of solids Page 1 of 8 Elastic Properties of Solids (One or two weights) This is a rare experiment where you will get points for breaking a sample! The recommended textbooks and other
More informationHomework No. 1 MAE/CE 459/559 John A. Gilbert, Ph.D. Fall 2004
Homework No. 1 MAE/CE 459/559 John A. Gilbert, Ph.D. 1. A beam is loaded as shown. The dimensions of the cross section appear in the insert. the figure. Draw a complete free body diagram showing an equivalent
More information6. Bending CHAPTER OBJECTIVES
CHAPTER OBJECTIVES Determine stress in members caused by bending Discuss how to establish shear and moment diagrams for a beam or shaft Determine largest shear and moment in a member, and specify where
More informationChapter 12. Static Equilibrium and Elasticity
Chapter 12 Static Equilibrium and Elasticity Static Equilibrium Equilibrium implies that the object moves with both constant velocity and constant angular velocity relative to an observer in an inertial
More informationCHAPTER 6 MECHANICAL PROPERTIES OF METALS PROBLEM SOLUTIONS
CHAPTER 6 MECHANICAL PROPERTIES OF METALS PROBLEM SOLUTIONS Concepts of Stress and Strain 6.1 Using mechanics of materials principles (i.e., equations of mechanical equilibrium applied to a freebody diagram),
More informationAdvanced Structural Analysis EGF Section Properties and Bending
Advanced Structural Analysis EGF316 3. Section Properties and Bending 3.1 Loads in beams When we analyse beams, we need to consider various types of loads acting on them, for example, axial forces, shear
More informationDAMAGE MECHANICS MODEL FOR OFFAXIS FATIGUE BEHAVIOR OF UNIDIRECTIONAL CARBON FIBERREINFORCED COMPOSITES AT ROOM AND HIGH TEMPERATURES
DAMAGE MECHANICS MODEL FOR OFFAXIS FATIGUE BEHAVIOR OF UNIDIRECTIONAL CARBON FIBERREINFORCED COMPOSITES AT ROOM AND HIGH TEMPERATURES M. Kawai Institute of Engineering Mechanics University of Tsukuba,
More informationModelling of the bullet perforation of textile targets
Structures Under Shock and Impact IX 355 Modelling of the bullet perforation of textile targets R. Barauskas 1, A. Abraitiene 2 & A. Vilkauskas 1 1 Department of System Analysis, Kaunas University of Technology,
More informationThe Relationship between the Applied Torque and Stresses in PostTension Structures
ECNDT 6  Poster 218 The Relationship between the Applied Torque and Stresses in PostTension Structures Fui Kiew LIEW, Sinin HAMDAN * and Mohd. Shahril OSMAN, Faculty of Engineering, Universiti Malaysia
More informationFIBRE WAVINESS INDUCED BENDING IN COMPRESSION TESTS OF UNIDERECTIONAL NCF COMPOSITES
FIBRE WAVINESS INDUCED BENDING IN COMPRESSION TESTS OF UNIDERECTIONAL NCF COMPOSITES Dennis Wilhelmsson 1, Leif E. Asp 1, Renaud Gutkin 2, Fredrik Edgren 3 1 Chalmers University of Technology, Dept. Industrial
More informationStatic and kinetic frictional characteristics of staple fibres and woven fabrics
Indian Journal of Fibre & Textile Research Vol. 32, March 2007, pp. 8087 Static and kinetic frictional characteristics of staple fibres and woven fabrics A Das a & S M Ishtiaque Department of Textile
More informationSTRAIN GAUGES YEDITEPE UNIVERSITY DEPARTMENT OF MECHANICAL ENGINEERING
STRAIN GAUGES YEDITEPE UNIVERSITY DEPARTMENT OF MECHANICAL ENGINEERING 1 YEDITEPE UNIVERSITY ENGINEERING FACULTY MECHANICAL ENGINEERING LABORATORY 1. Objective: Strain Gauges Know how the change in resistance
More informationSean Carey Tafe No Lab Report: Hounsfield Tension Test
Sean Carey Tafe No. 366851615 Lab Report: Hounsfield Tension Test August 2012 The Hounsfield Tester The Hounsfield Tester can do a variety of tests on a small testpiece. It is mostly used for tensile
More informationJeff Brown Hope College, Department of Engineering, 27 Graves Pl., Holland, Michigan, USA UNESCO EOLSS
MECHANICS OF MATERIALS Jeff Brown Hope College, Department of Engineering, 27 Graves Pl., Holland, Michigan, USA Keywords: Solid mechanics, stress, strain, yield strength Contents 1. Introduction 2. Stress
More informationChapter 3. Load and Stress Analysis
Chapter 3 Load and Stress Analysis 2 Shear Force and Bending Moments in Beams Internal shear force V & bending moment M must ensure equilibrium Fig. 3 2 Sign Conventions for Bending and Shear Fig. 3 3
More informationRESEARCH PROJECT NO. 26
RESEARCH PROJECT NO. 26 DETERMINATION OF POISSON'S RATIO IN AD1 TESTING BY UNIVERSITY OF MICHIGAN REPORT PREPARED BY BELA V. KOVACS and JOHN R. KEOUGH \ MEMBER / / DUCTILE IRON \ SOCIETY Issued by the
More informationTable of Contents. Preface...xvii. Part 1. Level
Preface...xvii Part 1. Level 1... 1 Chapter 1. The Basics of Linear Elastic Behavior... 3 1.1. Cohesion forces... 4 1.2. The notion of stress... 6 1.2.1. Definition... 6 1.2.2. Graphical representation...
More informationMECE 3321: Mechanics of Solids Chapter 6
MECE 3321: Mechanics of Solids Chapter 6 Samantha Ramirez Beams Beams are long straight members that carry loads perpendicular to their longitudinal axis Beams are classified by the way they are supported
More informationM98P2 (formerly C98P1) NonNewtonian Fluid Flow through Fabrics Matthew W. Dunn Philadelphia University
1 NonNewtonian Fluid Flow through Fabrics Matthew W. Dunn Philadelphia University http://spike.philacol.edu/perm/ Goal Statement The overall objectives of this program are to Model fabric porosity based
More informationHIGH VELOCITY IMPACT ON TEXTILE REINFORCED COMPOSITES
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS HIGH VELOCITY IMPACT ON TEXTILE REINFORCED COMPOSITES Warnet L., Akkerman R., Ravensberg M. University of Twente, Faculty of Engineering Technology,
More informationPLAIN WEAVE REINFORCEMENT IN C/C COMPOSITES VISUALISED IN 3D FOR ELASTIC PARAMETRES
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS PLAIN WEAVE REINFORCEMENT IN C/C COMPOSITES VISUALISED IN 3D FOR ELASTIC PARAMETRES P. Tesinova Technical University of Liberec, Faculty of Textile
More informationRESPONSE SURFACES OF MECHANICAL BEHAVIOR OF DRY WOVEN FABRICS UNDER COMBINED LOADINGS
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS RESPONSE SURFACES OF MECHANICAL BEHAVIOR OF DRY WOVEN FABRICS UNDER COMBINED LOADINGS M. Komeili, A.S. Milani* School of Engineering, University
More informationUnit I Stress and Strain
Unit I Stress and Strain Stress and strain at a point Tension, Compression, Shear Stress Hooke s Law Relationship among elastic constants Stress Strain Diagram for Mild Steel, TOR steel, Concrete Ultimate
More informationMECHANICS LAB AM 317 EXP 3 BENDING STRESS IN A BEAM
MECHANICS LAB AM 37 EXP 3 BENDING STRESS IN A BEAM I. OBJECTIVES I. To compare the experimentally determined stresses in a beam with those predicted from the simple beam theory (a.k.a. EulerBernoull beam
More information3D Elasticity Theory
3D lasticity Theory Many structural analysis problems are analysed using the theory of elasticity in which Hooke s law is used to enforce proportionality between stress and strain at any deformation level.
More informationModeling of FiberReinforced Membrane Materials Daniel Balzani. (Acknowledgement: Anna Zahn) Tasks Week 2 Winter term 2014
Institute of echanics and Shell Structures Faculty Civil Engineering Chair of echanics odeling of FiberReinforced embrane aterials OOC@TU9 Daniel Balani (Acknowledgement: Anna Zahn Tasks Week 2 Winter
More informationComposite Structures. Indian Institute of Technology Kanpur
Mechanics of Laminated Composite Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 23 Analysis of an Orthotropic Ply Lecture Overview Introduction Engineering constants for an 2
More informationFeatures and design of elastomer / textile engineered structures. D Boast, C Eng. F Mech E.
Features and design of elastomer / textile engineered structures D Boast, C Eng. F Mech E. Title of meeting IOM Bla blah Topics Materials: Environmental acids, water, oil, radiation etc. Bonding. Cost.
More informationChapter 7. Highlights:
Chapter 7 Highlights: 1. Understand the basic concepts of engineering stress and strain, yield strength, tensile strength, Young's(elastic) modulus, ductility, toughness, resilience, true stress and true
More informationEFFECT OF TEXTILE ARCHITECTURE ON ENERGY ABSORPTION OF WOVEN FABRICS SUBJECT TO BALLISTIC IMPACT
THE 9 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS EFFECT OF TEXTILE ARCHITECTURE ON ENERGY ABSORPTION OF WOVEN FABRICS SUBJECT TO BALLISTIC IMPACT C. Yang,*, P. Tran, T. Ngo, P. Mendis, B. Humphries
More informationStrength of Materials (15CV 32)
Strength of Materials (15CV 32) Module 1 : Simple Stresses and Strains Dr. H. Ananthan, Professor, VVIET,MYSURU 8/21/2017 Introduction, Definition and concept and of stress and strain. Hooke s law, StressStrain
More informationTensile stress strain curves for different materials. Shows in figure below
Tensile stress strain curves for different materials. Shows in figure below Furthermore, the modulus of elasticity of several materials effected by increasing temperature, as is shown in Figure Asst. Lecturer
More informationElastic parameters prediction under dynamic loading based on the. unit cell of composites considering end constraint effect
Elastic parameters prediction under dynamic loading based on the unit cell of composites considering end constraint effect Wang Meng 1,, Fei Qingguo 1,, Zhang Peiwei 1, (1. Institute of Aerospace Machinery
More informationChapter 5 Elastic Strain, Deflection, and Stability 1. Elastic StressStrain Relationship
Chapter 5 Elastic Strain, Deflection, and Stability Elastic StressStrain Relationship A stress in the xdirection causes a strain in the xdirection by σ x also causes a strain in the ydirection & zdirection
More informationObjective Evaluation of the Handle of Woven Terry Fabrics. Diana Krasteva, Deputy Head of Department, Textile Department Technical University of Sofia
Objective Evaluation of the Handle of Woven Terry Fabrics Diana Krasteva, Deputy Head of Department, Textile Department Technical University of Sofia Galya Kandzhikova Textile Department Technical University
More informationOutline. TensileTest Specimen and Machine. StressStrain Curve. Review of Mechanical Properties. Mechanical Behaviour
TensileTest Specimen and Machine Review of Mechanical Properties Outline Tensile test True stress  true strain (flow curve) mechanical properties:  Resilience  Ductility  Toughness  Hardness A standard
More informationMODELING OF THE BEHAVIOR OF WOVEN LAMINATED COMPOSITES UNTIL RUPTURE
MODELING OF THE BEHAVIOR OF WOVEN LAMINATED COMPOSITES UNTIL RUPTURE Jean Paul Charles, Christian Hochard,3, Pierre Antoine Aubourg,3 Eurocopter, 375 Marignane cedex, France Unimeca, 6 rue J. Curie, 3453
More informationTRESS  STRAIN RELATIONS
TRESS  STRAIN RELATIONS Stress Strain Relations: Hook's law, states that within the elastic limits the stress is proportional to t is impossible to describe the entire stress strain curve with simple
More informationANALYSIS OF YARN BENDING BEHAVIOUR
ANALYSIS OF YARN BENDING BEHAVIOUR B. Cornelissen, R. Akkerman Faculty of Engineering Technology, University of Twente Drienerlolaan 5, P.O. Box 217; 7500 AE Enschede, the Netherlands b.cornelissen@utwente.nl
More informationDEFORMATION PATTERN AND FAILURE CRITERIA OF WOVEN COMPOSITE PREFORM IN GENERAL BIAS EXTENSION
DEFORMATION PATTERN AND FAILURE CRITERIA OF WOVEN COMPOSITE PREFORM IN GENERAL BIAS EXTENSION B. Zhu 1,2*, T.X. Yu 1, X.M. Tao 2 1 Department of Mechanical Engineering, Hong Kong University of Science
More informationAnisotropy of the Static Friction. of Plainwoven Filament Fabrics
Anisotropy of the Static Friction of Plainwoven Filament Fabrics By Masayasu Ohsawa and Satoru Nam iki, Members, T M S J Faculty of Technology, Tokyo University of Agriculture and Technology, Koganei,
More informationWORKBOOK MECHANICS OF MATERIALS AND ELEMENTS OF ENGINEERING STRUCTURES
WORKBOOK MECHANICS OF MATERIALS AND ELEMENTS OF ENGINEERING STRUCTURES LUBLIN 014 Authors: Sylwester Samborski, Andrzej Teter and Marcin Bocheński Desktop publishing: Sylwester Samborski, Andrzej Teter
More informationA Novel Approach for Measurement of Fiberonfiber Friction
F98S09 Page 1 A Novel Approach for Measurement of Fiberonfiber Friction Number: F98S09 Competency: Fabrication Team Leader and members: Y. Qiu, NCSU; Y. Wang, Georgia Tech; J.Z. Mi, Cotton Inc. Graduate
More information